Assessment of natural radioactivity in various
commercial tiles used for building purposes in
, O.O. Adewoyina
, Z. Embongc
, F. Oyawoyed a
Department of Physics, Covenant University Ota, Nigeria
bDepartment of Chemistry, Covenant University Ota, Nigeria
cFaculty of Applied Science and[70_TD$DIFF]Teknologi, Universiti Tun Hussein Onn, Malaysia Pagoh Campus. km 1,
Jalan Panchor 84600, Muar, Johor, Malaysia
Department of Geosciences, University of Lagos, Nigeria
G R A P H I C A L A B S T R A C T
The tile samples were analyzed using High purity Germanium Gamma Detector.
Total numbers of 15 samples of various tiles which include foreign and locally produced were used for this study.
Evaluation of the activity concentration of natural radionuclides (226Ra, 232Th and 40K).
Various hazard indices were determined.
The mean activity concentrations of
226Ra, 232Th, and 40K
A B S T R A C T
In this study, we evaluated the activity concentration of natural radionuclides (226Ra,232Th and40K) forﬁfteen
(15) different brands of tile samples used for building purposes in Nigeria. The tile samples were analyzed using High purity Germanium gamma detector. The mean activity concentrations of226Ra,232Th, and40K were observed
to be 61.15.5 Bq/kg, 70.26.08 Bq/kg and 514.759.8 Bq/kg respectively. Various hazard indices such as absorbed dose rate, external and internal hazard index, annual effective dose rate, Gamma activity Index (Ig) and Alpha Index (Ia) were calculated. The obtained results showed that the mean radium equivalent activity (Raeq), the absorbed dose rate (D), external and internal hazard index, the annual effective dose (AEDR) equivalent, Gamma activity Index (Ig) and Alpha Index (Ia) were: 204.42 Bq/kg, 177.61 nGyh1, 0.55, 0.77, 0.96 mSvyr1,
0.74 and 0.32 respectively. The average value of radium equivalent obtained in this study is less than that of the
* Corresponding author at: Department of Physics, Covenant University Ota, Nigeria.
E-mail addresses:firstname.lastname@example.org(E.S. Joel),email@example.com
2215-0161/© 2018 Published by Elsevier B.V. This is an open access article under the CC BY license (http://creativecommons.org/
Contents lists available atScienceDirect
recommended value of 370 Bq/kg but the average values of the other radiological hazards for some samples are found to be slightly above international recommended values except Hex, Hinand AEDE which are within the
international reference value of unity. The measured concentrations of these radioactive materials were correlated with other previous result obtained from similar tile materials used in other countries and found to be in good agreement with the international standard, however, the tiles are recommended for decoration purposes in Nigeria.
© 2018 Published by Elsevier B.V. This is an open access article under the CC BY license (http://creativecommons. org/licenses/by/4.0/).
A R T I C L E I N F O
Keywords:Radionuclides, Tiles, Hazard indices, Annual effective dose rate
Article history:Received 21 September 2017; Accepted 6 December 2017; Available online 4 January 2018
Humans society have always been exposed on daily basis to natural radionuclides such as232Th,
Ra and40K[72_TD$DIFF]. These radionuclides in the series are headed by226Ra (238U) and are relatively less
important from a dosimetric point of view[73_TD$DIFF]. The origin of these materials is the Earth's crust, but
theyﬁnd their way into building materials, air, water, food and the human body itself. The world wide
average indoor effective dose due to gamma rays from building materials is estimated to be about 0.4
mSv per year[74_TD$DIFF][3,4]. Globally, building materials that contain radioactive nuclides have been used for
many decades. As individuals spend more than 80% of their time indoors, the internal and external
radiation exposure from building materials creates prolonged exposure situations[75_TD$DIFF]. The external
radiation exposure is caused by the gamma emitting radionuclides, which in the uranium series
mainly belongs to the decay chain segment starting with226Ra. The internal (inhalation) radiation
exposure is due to222Rn, and marginally to220Rn, and their short lived decay products, exhaled from
building materials into the room air[76_TD$DIFF]. Papastefanou et al.[77_TD$DIFF] carried out a study in Greece on
building materials, which showed that out of the investigated building materials such as tiles which are by product of granite, phosphogypsum etc. are highly radioactive materials for which the absorbed
dose rate in indoor air becomes up toﬁve times higher than the dose criterion. Such radioactive
materials contribute signiﬁcantly to radiation exposure because they comprise gamma and beta
emitters [78_TD$DIFF][7,1]. Building materials, derived from rock, sand, soil and byproduct of industry, often
contain varying amounts of natural radionuclides[79_TD$DIFF][8–10]. The knowledge of the natural radioactivity
level of building materials is important for determination of population exposure to radiation. Furthermore, knowledge of this radioactivity is useful in setting the standards and national guidelines for the use and management of these materials and in assessing the associated radiation hazard to
human health [80_TD$DIFF]. The natural radioactivity level of building materials can vary considerably
according to the geological locations and geochemical characteristics of those materials. Due to the increasing social concern, the natural radioactivity level of building materials has been reported in
many countries [81_TD$DIFF][12–22]. The objectives of the study are to evaluate the activity concentration of
natural radioactivity content in the commonly used building materials such as tiles of various types and sizes in Nigeria and to estimate the radiation hazards associated to individuals by using radium equivalent activity, external and internal hazard indexes, indoor air absorbed dose rate and annual effective dose rate. The results are compared with the internationally reference values to ascertain the safer tiles useful for building purpose in Nigeria.
Materials and methods
Total numbers of 15 samples of various tiles which include foreign and locally produced were used for this study. These tiles are Virony (china), Gomez (Spain), BN Ceramics (Nigeria), Virony Rustic (China), PNT Ceramics (Nigeria), Pamesa (Spain), Virony (China), Virony (China) Rustic Glass, Iris (Italy), Golden Crown Ceramics (Nigeria), Royal Ceramics (Nigeria), Royal Crown(Nigeria), Goodwill
Super Polish (Nigeria), BN Ceramics (Spain) and Goodwill Ceramics (Nigeria). This is shown inTable 1
with their sample names, sample ID and country. The tiles samples used for this work were purchased from the Nigerian commercial markets. Initial labeling and cataloguing was done for easy
identiﬁcation. The tiles were broken into smaller pieces so as to allow further processing. All the
samples were crushed using the Pascall Engineering Lab milling machine to pulverizable size. After each tile sample was crushed, the crusher or lab milling machine was thoroughly cleaned with high pressure blower (Wolf from Kango Wolf power tools, made in London, type 8793 and serial no: 978A) before the next sample was crushed, to avoid cross contamination of the samples.
A veryﬁne power was achieved from the pulverized samples, but for homogeneity, a 250
size was used and 1 kg of the sieved sample was weighed out. It was then placed in polythene nylon and labeled accordingly. High density polyethylene bottles (HDPB) were used to package the samples for radioactivity study. The bottles were washed with water and detergent and then rinsed six times
with ordinary borehole water beforeﬁnally rinsing with distilled water. The sieved samples of tiles
that were contained in each bottle weighed 200 g.
Gamma ray detection system for this study
The analysis was carried out using the gamma ray spectrometry facilities at the Nuclear Lab. Faculty of Science, Universiti Teknologi Malaysia. A high resolution spectrometer was used for the measurement of the gamma energy spectrum of emitted gamma-rays in the energy range between 50 keV and 2000 keV. The gamma ray spectrometry consists of a high purity germanium (HPGe)
detector with a counting efﬁciency of 20%, a resolution of 1.8 keV for 1332 keV gamma ray emission of
60Co. The detector used in gamma ray measurements was Canberra GC2018 with Genie-2000 software.
The gamma detector was cooled by liquid nitrogen at 77 K for the purpose of reducing leakage current and thermal noise, and its warm-up sensor is coupled to the high voltage detector bias supply. The
pre-ampliﬁer was placed inside a lead shield to reduce background radiation[82_TD$DIFF]. The decay isotopes,
gamma energy and gamma disintegrations are shown inTable 2.
Tiles of different types and country of origin used in Nigeria.
Sample Name Country Sample ID
Virony China 4040
Gomez Spain 4040
BN Ceramics Nigeria 6060
Virony Rustic China 4040
PNT Ceramics Nigeria 3030
Pamesa Spain 600300
Virony China 3030
Virony Rustic Glass China 4040
Iris Italy 33.333.3
Golden Crown Ceramics Nigeria 2530
Royal Ceramics Nigeria 4040
Royal Crown Nigeria 3030
Goodwill Super Polish Nigeria 6060
BN Ceramics Spain 4545
Standard sample preparation for gamma spectrometry
The IAEA standard sample Thorium Ore (S-14) and Lake Sediment (SL-2) were used as reference
materials and mixed with SiO2in Marinelli beakers. The Uranium and Thorium contents from S-14 are
29 ppm and 610 ppm respectively. A weight of 20.00 g from Sample IAEA S-14 was thoroughly mixed
with 100.00 g of SiO2in a Marinelli beaker (Coded as S-14). After mixing with SiO2, the Uranium and
Thorium concentrations are 4.63 ppm and 97.3 ppm respectively. The IAEA standard sample
SL-2 was used to calculate the speciﬁc activity of potassium (K). It has a speciﬁc activity of 240 Bq kg1.
Another Marinelli beaker containing a weight of 74.18 g of SL-2 was mixed with 100.00 g of SiO2
(Coded as SL-2). This provides background for standard samples. The IAEA standard samples used in
this study are presented inTable 3.
Calculation of238U and232Th in thorium ore (IAEA S-14) and40K in lake sediment (IAEA SL-2)
Theweightof measuredsampleusedf romS14¼20:00g
Concentrationof232ThinThoriumoreðS14Þ ¼610ppm ð2Þ
ð4Þ Table 2
The decay Isotopes, Gamma-ray Energy and Gamma disintegration.
Radioactive Series Decaying Isotopes Gamma-ray Energy (keV) Percentage of Gamma
U decay series) 352.0 35
214 Bi (for238
U decay series) 609.4 43
Thorium 208Tl (for232Th decay series) 583.1 30
Ac (for232Th decay series) 911.1 29
K 1460.8 10.68 or 11
IAEA standard samples used in this study.
Standard Sample Code Concentrations
U (ppm) Th (ppm) K (Bq/kg)
S-14 (Thorium ore) 29 610 –
SL-2 (Late sediment) – – 240
Measurement of gamma-ray radioactivity from the tiles samples used in this study
The tiles imported and produced in Nigeria of different brands purchased from different suppliers,
were prepared according to IAEA TRS-295[83_TD$DIFF]. The samples were sealed and stored for four weeks to
achieve secular equilibrium between radium and its progeny[84_TD$DIFF][25–29]. Under the conditions of secular
equilibrium,232Th concentration was determined from the average concentration of208Tl using the
583 keV peak and 228Ac by using the 911 keV peak. 238U was determined from the average
concentrations of the214Pb by using the 352 keV peak and214Bi by using the 609 keV peak[84_TD$DIFF][25–29]. The
1460 keV peak was used to determine the concentration of K. Each sample was put into a shielded HPGe detector and measured for 21600 s. The background gamma-ray spectrum of the detection system was determined with an empty Marinelli beaker under identical conditions, and was
subtracted from the spectra of each sample. The speciﬁc activity was determined by comparing with
IAEA standard samples S-14 (Thorium ore) and SL-2 (Lake Sediment). The concentration of the238U
and232Th was determined using Eqs.(5)and(6). Eqs.(7)and(8)were used for40K
Csamp= concentration of sample collected (ppm)
Cstd= concentration of the standard sample (ppm)
Wstd= weight of the standard sample (g)
Wsamp= weight of the sample collected (g)
Nsamp= net counts of the photopeak area of the sample collected
Nstd= net counts of the photopeak area of the standard sample.
The uncertainty of the sample concentration was calculated by using the accurate approach by[85_TD$DIFF]
Conversion factors were used to convert ppm to Bq kg1. [238U; 1 ppm = 12.35 Bq kg1;232Th;
1 ppm = 4.06 Bq kg1]. Whereas 1% of40K = 313 Bq kg1[86_TD$DIFF].
The speciﬁc activity of potassium was calculated by using the formula:
Asamp= the speciﬁc activity of the sample collected (Bq Kg1)
Astd= the speciﬁc activity of standard sample (Bq Kg1)
Wstd= the weight of the standard sample (Kg)
Nsamp= the net counts of the photopeak area for the sample collected
Wsamp= the weight of the sample collected (Kg)
Nstd= the net counts of the photopeak area for the standard sample.
The uncertainty of the speciﬁc activity of potassium was calculated by using the following formula:
Results and discussions
materials (226Ra,232Th and40K) and their mean activities are shown inTable 2. The measured mean
activity concentrations of226Ra,232Th and40K radionuclides in various tiles samples were observed to
be 61.15.5 Bq/kg, 70.26.08 Bq/kg and 514.759.8 Bq/kg respectively. Figs. 1–3 describe the
relationship between speciﬁc concentration activities of226Ra,232Th, and40K and the various tiles
samples respectively. FromTable 4, it was observed that activity concentration of226Ra of the sample
tiles ranged between 37.53.6 Bq/kg and 24125.3 Bq/kg with PNT ceramics tile having the highest
value of 24125.3 Bq/kg (Fig. 1), while the lowest concentration activity of226Ra is found in Pamesa
tile type sample (Spain) with value of 30.54.1 Bq/kg, followed by BN ceramic tile which is produced
in Nigeria where the activity concentration was 37.53.6 Bq/kg. Except for PNT ceramics tile, all other
tile samples are within the permissible value that ranged between 30 and 200 Bq/kg[87_TD$DIFF] for226Ra.
Highest concentration activities of232Th were found to be Virony tile type imported from China with
the value of 126.59.1 Bq/kg, followed by BNT ceramic tiles imported from Spain and BNT ceramic
Fig. 1. Concentrations of226
Ra for various tiles samples used for building in Nigeria.
Fig. 2.Concentrations of232Th for various tiles samples used for building in Nigeria.
Fig. 3.Concentrations of40
K for various tiles samples used for building in Nigeria.
tiles which was locally produced in Nigeria with values of 104.58.3 Bq/kg and 101.58.2 Bq/kg
respectively. The lowest232Th activity concentration was found to be Royal crown tile (Nigeria) with
value of 413.6 Bq/kg.Fig. 3shows the highest values of40K activity which are 940115.1 and
65081.4 Bq/kg for tile samples Iris and Pamesa from Italy and Spain respectively. Comparing the
concentration activity value of40K with the[87_TD$DIFF] report, it shows that the values are within permissible
value of 160–1410 Bq/kg. A comparative analysis with the previous investigation conducted in
different parts of the world has been shown inTable 5.
Exposure risk assessment
Radioactivity equivalent (Raeq)
The radionuclides distribution such as 226Ra, 232Th and 40K in tiles are not homogeneous.
Comparing the concentrations and assessing the health risk hazard of the tile materials, the
radioactive activity equivalent (Raeq). The radioactivity equivalent is deﬁned generally as 
Raeq = ACRA+ 1.43ACTh+ 0.077ACK (9)
Activity concentrations in Bq/kg of commercial tiles samples used in Nigeria.
Sample Name Sample size Activity Concentration (Bq/kg)
226Ra 232Th 40K
Virony (China) 4040 55.54.2 126.59.1 53065.1
Gomez (Spain) 4040 57.54.2 758.1 45052.1
BN Ceramics (Nig) 6060 37.53.6 101.58.2 67070.2
Virony Rustic (China) 4040 59.54.1 41.53.6 48052.1
PNT Ceramics 3030 24125.3 77.58.1 510.062.6
Pamesa (Spain) 600300 30.54.1 644.1 65081.4
Virony (China) 3030 554.2 524.2 44042.1
Virony (China) Rustic Glass 4040 42.53.6 634.1 39050.1
Iris (Italy) 33.333.3 59.54.2 798.3 940115.1
Golden Crown Ceramics (Nig) 2530 49.53.1 57.54.6 46050.4
Royal Ceramics (Nig) 4040 65.55.4 444.1 39050.2
Royal Crown 3030 51.53.7 413.9 44042.1
Goodwill Super Polish (Nig) 6060 443.6 51.54.5 27030.5
BN Ceramics (Spain) 4545 554.2 104.58.3 57067.3
Goodwill Ceramics (Nig) 4040 625.2 74.58.1 53065.1
Average concentration 61. 15.5 70.26.08 514.759.8
Range 30.5–241.0 41.5–126.5 270.0–940.0
Comparative analysis of activity concentrations in Bq/kg of commercial tiles samples used in different countries.
Countries Activity Concentration (Bq/kg) Reference
Range Average Range Average Range Average
Pakistan 63.1–123.9 83.4 – – 144.1–834 403.5 [57_TD$DIFF]
Egypt (Lecico and El-Gawhra) 41.7–60.7 52.2 30.7–47.1 39.1 195–680 480 [58_TD$DIFF]
Qena (Egypt) 40–230 126 10–130 72 80–600 300 [59_TD$DIFF]
Algeria 55 – 41 – 410 [60_TD$DIFF]
Egypt (Cleopatra Factory) 71.2–86 76.1 63.3–68.7 66.2 900–1018 962 [61_TD$DIFF]
China 63.5–131.4 – 55.4–106.5 – 63.5–131.4 – [62_TD$DIFF]
Italy – 56 – 43 – 440 [63_TD$DIFF]
Cameroon 11.3–13.13 12 18.63–22.64 20 – 319 [64_TD$DIFF]
Palestine 45.4–102.0 73.7 38.8–78.3 58.2 363–871.2 624 [65_TD$DIFF]
Yemen 0–549 131.88 13–267 83.55 24–869 400.7 [66_TD$DIFF]
where ACRA, ACThand ACKare the activity concentrations of226Ra,232Th and40K respectively in Bq/kg.
Eq.(9)is based on the fact that 370 Bq/kg of226Ra, 259 Bq/kg of232Th and 4810 Bq/kg of40K produce
the same gamma ray dose equivalent[88_TD$DIFF]. The maximum value of Radioactivity equivalent must be
less than 370 Bq/kg in order to maintain the external dose <1.5 mGy/yr [89_TD$DIFF]. The values of
radioactivity equivalent are shown in Table 6. The measured value ranged between138.44 and
391.10 Bq/kg with mean value of 204.42 Bq/kg which is less than the recommended value of 370 Bq/kg
by UNSCEAR[90_TD$DIFF] and International Atomic Energy Agency[91_TD$DIFF].
Absorbed dose rate
The indoor air absorbed dose rate (D) as a result of emission of gamma ray from the natural
radioactive materials in the building materials (such as tiles) is estimated based on the[92_TD$DIFF] report as
shown in Eq.(10)
D(nGyh1) = 0.92C
Ra+ 1.1CTh+ 0.08Ck (10)
where CRa, CThand Ckthe activity concentration of226Ra,232Th and40K respectively in Bq/kg. The value
obtained for absorbed rate ranged from 118.73 to 347.77 nGyh1as shown inTable 6with average
value of 177.61 nGyh1. It was observed that PNT ceramic tile have the highest absorbed dose rate of
347.77 nGyh1 while Goodwill super polish tile have the lowest value of 118.73 nGyh1 for the
absorbed dose rate. Further observation shows that the values of absorbed dose rate for the entire
sample tiles are more than the recommended value of 55 nGyh1 [93_TD$DIFF] and 84 nGyh1 by 
External and internal hazard index
Exposure of radiation due to radionuclides such as 226Ra,232Th and 40K may be external and
internal. The hazard which is deﬁned in relation to external and internal hazard is represented by Hex
and Hinrespectively and can be determined using Eqs.(11)and(12)[94_TD$DIFF]:
Hin= (CRa/370) + (CTh/259) + (CK/4810) (11)
Hex= (CRa/185) + (CTh/259) + (CK/4810) (12)
where CRa, CThand CKare activity concentrations of226Ra,232Th and40K, respectively in Bq/kg. The
index value for Eq.(11) should be less than 1 or negligible in order for the external hazard to be
Radiation indices of the various tiles samples used in Nigeria.
Sample No. Sample Name Raeq(Bq/kg) D(nGyh1) Hex Hin AEDR (mSv/yr)
17 Virony (China) 277.21 232.61 0.75 0.89 1.30
18 Gomez (Spain) 199.40 171.40 0.54 0.69 0.94
19 BN Ceramics 234.24 199.75 0.63 0.73 1.12
20 Virony Rustic (China) 155.81 138.79 0.42 0.58 0.73
21 PNT Ceramics 391. 10 347.77 1.06 1.71 1.77
22 Pamesa (Spain) 172.07 150.46 0.47 0.55 0.83
23 Virony (China) 163.24 143.00 0.44 0.59 0.77
24 Virony (China) Rustic Glass 162.62 139.60 0.44 0.55 0.77
25 Iris (Italy) 244.85 216.84 0.66 0.82 1. 18
26 Golden Crown Ceramics (Nigeria) 167.15 145.59 0.45 0.59 0.79
27 Royal Ceramics (Nigeria) 158.45 139.86 0.43 0.61 0.74
28 Royal Crown (Nigeria) 144.01 127.68 0.39 0.53 0.68
29 Goodwill Super Polish (Nigeria) 138.44 118.73 0.37 0.49 0.65
30 BN Ceramics (Spain) 248.33 211.15 0.67 0.82 1. 17
31 Goodwill Ceramics (Nigeria) 209.35 181.39 0.57 0.73 0.99
32 Average 204.42 177.61 0.55 0.73 0.96
Range 138.44–391. 10 118.73–
acceptable to the public[89_TD$DIFF]. The maximum value of unity for Hexcorresponds to the limit 370 Bq/kg
for Radioactivity equivalent. For the safe use of a building material in the dwellings construction, Hin
should be less than unity. The calculated values of the Hexand Hinfor tile samples used are shown in
Table 6. The values ranged between 0.37 and 1.06 with mean value of 0.55 for external hazard (Hex)
while the values for internal hazard (Hin) range from 0.49 to 1.71. The obtained result for Hexfor PNT
ceramic tile is above recommended limit of unity as well as Hin which is almost twice the
recommended value. The results for other tile samples are less than unity and are in agreement with the recommended international values.
Annual effective dose rate
In determining the annual effective dose, the coefﬁcient of conversion factor (0.7SvGy1) from the
absorbed dose in air to the effective dose received by individual and the indoor occupancy factor 0.8 as
proposed by[90_TD$DIFF] are used. The annual effective dose rate (AED) is calculated using Eq.(13):
AEDR(mSvy1) =D(nGyh1)8760 (h)0.80.7 (SvGy1)106 (13)
The annual effective dose rate of the tiles used for this study is shown inTable 6which ranged from
0.65–1.77 mSvy1but it was observed that some samples such as Virony (China), BN ceramic (Nigeria),
PNT ceramics (Nigeria), Iris (Italy) and BN ceramic (Spain) have values of 1.30 mSv/yr, 1.12 mSv/yr, 1.77 mSv/yr, 1.18 mSv/yr and 1.17 mSv/yr respectively, which exceeded international standard value of 1 mSv/yr while other samples are within the recommended value. It was further observed that
concentration of232Th and40K might have contributed to the high annual effective dose rate value
observed in Virony tile sample while226Ra and 40 K,232Th and40K,40K,232Th and40K contributed to
the other tiles samples whose annual effective dose rate is higher than higher the recommended value of 1 mSv/yr.
Gamma index determination (I
Gamma index is used to evaluate the
g-radiation hazard related to the natural radionuclide in the
particular samples under investigation. The gamma index representation (I
g) is estimated using
Eq.(6)as presented by[95_TD$DIFF].
g=CRa/300 (Bqkg1) + CTh/200 (Bqkg1) + CK/3000 (Bqkg1) (14)
The estimated results are presented in Table 7. The controls on the radioactivity of building
materials according to RP122[92_TD$DIFF] is based on the dose criterion for control and exemption. The dose
Gamma activity and alpha indices of the various tiles samples used in Nigeria.
Sample No. Sample Name Gamma activity Index(Ig)(Sv yr1
) Alpha Index (Ia)
17 Virony (China) 0.99 0. 28
18 Gomez (Spain) 0.72 0. 29
19 BN Ceramics 0.86 0.19
20 Virony Rustic (China) 0.57 0. 29
21 PNT Ceramics 1.36 1.21
22 Pamesa (Spain) 0.64 0.15
23 Virony (China) 0.59 0.28
24 Virony (China) Rustic Glass 0.58 0.21
25 Iris (Italy) 0.91 0. 29
26 Golden Crown Ceramics (Nigeria) 0.61 0.24
27 Royal Ceramics (Nigeria) 0.57 0.32
28 Royal Crown (Nigeria) 0.52 0. 26
29 Goodwill Super Polish (Nigeria) 0.49 0.22
30 BN Ceramics (Spain) 0.89 0.28
31 Goodwill Ceramics (Nigeria) 0.76 0.31
32 Average 0.74 0.32
effective that is above the criterion level of 1 mSvy1should be taken into consideration for radiation protection. It is generally recommended that effective doses due to building materials should not
exceed 1 mSvy1with respect to the outdoor background. Higher doses should be accepted only in
highly speciﬁc circumstances where materials are locally used. For excess doses in the range 0.3–
1 mSvy1, controls are recommend, while building materials should be exempted from all restrictions,
concerning their radioactivity, if the excess gamma radiation originated from them increases the annual effective dose of a member of the public by 0.3 mSv at the most. The gamma activity index is
used to identify whether a dose criterion is met[96_TD$DIFF]. This gamma activity index accounts for the ways
and amounts in which the materials used in building, with limit value of their indices not exceeding
the recommended value and depends on the dose criterion shown inTable 7. The gamma activity
index1 corresponds to annual effective dose less than or equal to 1 mSvy1, while gamma activity
index0.5 corresponds to 0.3 mSvy1if the materials are used in bulk quantity. At the same time,
gamma activity index6 corresponds to annual effective dose of 1 mSvy1and gamma activity index
6 2 corresponds to an annual effective dose0.3 mSvy1for superﬁcial materials such as tiles which
is made in Nigeria vary from 0.49 mSvy1(Goodwill Super Polish) to 1.36 mSvy1(PNT ceramics) with
average value of 0.74 mSvy1. All the values presented here are below the criterion which corresponds
to the protection level of effective maximum dose of 1 mSv, except PNT ceramic.
Determination of alpha index (I
The assessment of the alpha index is another important aspect of hazard assessment that deals with the estimation of that excess alpha radiation due to radon inhalation originating from building
materials. The alpha index calculated using Eq.(15)[97_TD$DIFF][38,7] is:
a=CRa/200 (Bqkg1) (15)
where CRais the activity concentration of radium Bqkg1in building materials. If the radium activity
level in building material exceeds the values of 200 Bqkg1 there is possibility that the radon
exhalation from the material could cause indoor radon concentrations exceeding Bqm3.Table 5
present the values for alpha index. The International Commission on Radiation Protection (ICRP)
recommends an activity level of 200 Bqm3for radon in dwellings[98_TD$DIFF]. At the same time, if this
radium activity level is below 100 Bqkg1, it shows that radon exhalation from building materials may
not likely cause indoor concentration greater than 200 Bqm3[99_TD$DIFF]. It is reported that the recommended
exempted value and the recommended upper limit for radon concentrations are 100 Bqkg1 and
200 Bqkg1 respectively in building materials
. It is noted that the upper limit of radon
a) is equal to 1 [101_TD$DIFF]. The results of the present study show that the radon
concentration varies from 0.19 to 1.21 respectively with average value of 0.32 for the tiles used in Nigeria.
The measurement of natural radionuclides and its associated radiological hazards from 15 investigated tiles samples used in Nigeria for buildings purposes were evaluated using gamma ray spectrometry. The following conclusions can be drawn:
1. The mean activity concentration of226Ra,232Th and40K have been found to be in the range of
30.54.1–241.025.3, 41.53.6–126.59.1 and 27030.5–940115.1 Bq/kg respectively. On
the average, activity concentration of226Ra,232Th and40K were found to be below recommended
2. The radium equivalent activity for most of the tiles samples used is less than the recommended
value of 370 Bq/kg set in by[90_TD$DIFF] report except PNT ceramic tile sample with a value of 391. 10 Bq/kg.
3. The absorbed dose rate in air was found to range from 118.73 to 347.77 nGyh1with mean value of
177.61 nGyh1, which is higher than international values of 55 nGyh1according to[102_TD$DIFF] and 84
nGyh1according to[90_TD$DIFF] by a factor of 3.2 and 2.1, respectively.
4. The average value of Hex and Hinare 0.55 and 0.73 respectively which is lower than unity as
recommended by[90_TD$DIFF][56_TD$DIFF] except for tile sample PNT ceramic.
5. The result of annual effective dose rate show higher value in tile samples Virony (China), BN ceramic (Nigeria), PNT ceramic (Nigeria), Iris (Italy), BN ceramic (Spain) above recommended value of 1 mSv/yr but on the average value the annual effective dose rate is within the recommended limit. From the above result, it shows that the imported tiles such as Virony china, Iris (Italy) and BN ceramics (Spain) for building purposes should be monitored for other materials before a comprehensive conclusion will be drawn for its usage in Nigeria.
6. The mean values of gamma activity index and alpha index for the tiles used in Nigeria are
0.74 Sv yr1 and 0.32 Sv yr1 respectively except for the PNT ceramics and this tile should be
monitored before usage for building purposes.
The researchers appreciate Covenant University Ota for the grants given to embark on this research for the safety of our nation through Research Management Center Grant Scheme Number: CUCRID/VC/ 17/02/02/06-FS. Also, appreciation goes to Radiation Geophysics Research Group, Department of
Physics, Covenant University Ota, for their scientiﬁc contribution to this work.
S.A. Amin, M. Naji, Natural radioactivity in different commercial ceramic samples used in Yemeni buildings, Radiat. Phys.
Chem. 86 (2013) 37–41.
UNSCEAR, Exposure From Natural Sources of Radiation. Report to the General Assembly, UN, New York, 1993.
UNSCEAR, Sources, Effects, and Risks of Ionizing Radiation. Report to the General Assembly, with Scientiﬁc Annexes, UN,
New York, 2000.
N. Sharma, J. Singh, S.C. Esakki, R.M. Tripathi, A study of the natural radioactivity and radon exhalation rate in some
cements used in India and its radiological signiﬁcance, J. Radiat. Res. Appl. Sci. (2016) 47–56.
ICRP, Protection of the public in situations of prolonged radiation exposure, Ann. ICRP 29 (1–2) (1999) (Publication 82,
Elsevier Sciences, B.V. International Commission on Radiological Protection).
C. Papastefanou, S. Stoulos, M. Manolopoulou, The radioactivity of building materials, J. Radioanal. Nucl. Chem. 266 (2005)
L. Xinwei, W. Lingqing, J. Xiaodan, Y. Leipeng, D. Gelian, Speciﬁc activity and hazards of Archeozoic–Cambrian rock samples
collected from the Weibei area of Shaanxi, China, Radiat. Prot. Dosim. 118 (2006) 352–359.
A. Matiullah Ahad, S. Rehman, S. Rehman, M. Faheem, Measurement of radioactivity in the soil of Bahawalpur Division,
Pakistan, Radiat. Prot. Dosim. 112 (2004) 443–447.
S. Rahaman, A.S. Matiullah Mujahid, S. Hussain, Assessment of radiological hazards due to the presence of natural
radionuclides in samples of building materials collected from the northwestern areas of Pakistan, J. Radiol. Prot. 28 (2008)
J.M. Sharaf, M.S. Hamideen, Measurement of natural radioactivity in Jordanian building materials and their contribution to
the public indoor amma dose rate, Appl. Radiat. Isot. 80 (2013) 61–66.
X. Lu, S. Chao, G. Yang, Determination of natural radioactivity and associated radiation hazard in building materials used in
Weinan, China, Radiat. Phys. Chem. (2014) 62–67.
J. Beretka, P.J. Mathew, Natural radioactivity of Australian building materials, industrial waste sand by-products, Health
Phys. 48 (1985) 87–95.
M. Ngachin, M. Garavaglia, C. Giovani, M.G.K. Njock, A. Nourreddine, Assessment of natural radioactivity and associated
radiation hazards in some Cameroonian building materials, Radiat. Meas. 42 (2007) 61–67.
M. Faheem, S.A. Mujahid, Matiullah, Assessment of radiological hazards due to the natural radioactivity in soil and building
material samples collected from six districts of the Punjab province-Pakistan, Radiat. Meas. 43 (2008) 1443–1447.
A. El-Taher, S. Makhluf, A. Nossair, A.S. AbdelHalim, Assessment of natural radioactivity levels and radiation hazards due to
cement industry, Appl. Radiat. Isot. 68 (2010) 169–174.
H.H. Hussain, R.O. Hussain, R.M. Yousef, Q. Shamkhi, Natural radioactivity of some local building materials in the middle
Euphrates of Iraq, J. Radioanal. Nucl. Chem. 284 (2010) 43–47.
B. Mavi, I. Akkurt, Natural radioactivity and radiation hazards in some building materials used in Isparta, Turkey, Radiat.
Phys. Chem. 79 (2010) 933–937.
B.M. Moharram, M.N. Suliman, N.F. Zahran, S.E. Shennawy, A.R. ElSayed, External exposure doses due to gamma emitting
natural radionuclides in some Egyptian building materials, Appl. Radiat. Isot. 70 (2012) 241–248.
H. Al-Sulaiti, N. Alkhomashi, N. Al-Dahan, M. Al-Dosari, D.A. Bradley, S. Bukhari, M. Matthews, P.H. Regan, T.
Santawamaitre, Determination of the natural radioactivity in Qatarian building materials using high-resolution
gamma-ray spectrometry, Nucl. Instrum. Methods Phys. Res. A 652 (2011) 915–919.
N. Damla, U. Cevik, A.I. Kobya, A. Celik, N. Celik, I. Yıldırım, Assessment of natural radioactivity and mass attenuation
R. Ravisankar, K. Vanasundari, A. Chandrasekaran, A. Rajalakshmi, M. Suganya, P. Vijayagopal, V. Meenakshisundaram, Measurement of natural radioactivity in building materials of Namakkal, Tamil Nadu, India using gamma-ray
spectrometry, Appl. Radiat. Isot. 70 (2012) 699–704.
M.Ç. Tufan, T. Dişci, Natural radioactivity measurements in building materials used in Samsun, Turkey, Radiat. Prot. Dosim.
156 (2013) 87–92.
N. Tsoulfanidis, Measurement and Detection of Radiation, Taylor and Francis, 1995.
IAEA, Technical Reports, Series No: 295, International Atomic Energy Agency, 1989.
I. Alnour, H. Wagiran, N. Ibrahim, Z. Laili, M. Omar, S. Hamzah, B.Y. Idi, Natural radioactivity measurements in the granite
rock of quarry sites, Johor, Malaysia, Radiat. Phys. Chem. 81 (12) (2012) 1842–1847.
N.M. Ibrahim, Abd El, A.H. Ghani, S.M. Shawky, E.M. Ashraf, M.A. Faruk, Measurement of radioactivity level in soil in Nile
Delta and Middle Egypt, Health Phys. 4 (1993) 620–627.
O. Maxwell, H. Wagiran, N. Ibrahim, S.K. Lee, S. Soheil, Comparison of238
K in different layers of subsurface
structuresion Dei-Dei and Kubwa, Abuja, North Central Nigeria, Radiat. Phys. Chem. 91 (2013) 70–80.
B.S. Supian, C.J. Evans, Statistics and Nuclear Counting: Theory, Problems and Solutions Statistics and Errors in
Measurements, (1992) pp. 26–35.
International Atomic Energy Agency, Extent of Environmental Contamination by Naturally Occurring Radioactive Material
(NORM) and Technological Options for Mitigation, Technical Reports Series No. 419, STI/DOC/010/419, (2003).
M. Tufail, N. Ahmed, S. Almakky, M. Zafar, H. Khan, Natural radioactivity in the ceramic used in dwellings as construction
material, Sci. Total Environ. 127 (3) (1992) 243–253.
R. Higgy, Measurements and Analyses of Low Level Natural Radioactivity in Building Materials and Evaluation of Its
Environmental Impact. Ph.D. Thesis, Faculty of Science, Ain Shams University, Cairo, Egypt, 1995 pp. 130–136.
N. Ahmed, Measurements of natural radioactivity in building materials in Qena City—Upper Egypt, Proceedings of the 4th
Radiation Physics Conference, Alexandria—Egypt, 1999 pp. 15–191.
A. Amarani, M. Tahtat, Natural radioactivity in Algerian building materials, Appl. Radiat. Isot. 54 (4) (2001) 687–689.
M. Hilal, Nuclear Spectroscopic Measurements for Different Environmental Radiations. Ph.D. Thesis, Faculty of Science,
University of Mansoura, Egypt, 2002 (p. 138).
L. Xinwei, Radioactivity level in Chinese building ceramic tile, Radiat. Prot. Dosim. 112 (2) (2004) 323–327.
S. Righi, L. Bruzzi, Natural radioactivity and radon exhalation in building materials used in Italian dwellings, J. Environ.
Radioact. 88 (2006) 158–170.
K.M. Dabayneh, Natural radioactivity in different commercial ceramic samples used in Palestine buildings as construction
materials, Herbron Univ. Res. J. 3 (2) (2008) 49–58.
EC, Radiological protection principles concerning the natural radioactivity of building materials, Radiation Protection,
(1999) , pp. 112.
UNSCEAR, Sources, Effects and Risks of Ionizing Radiations, United Nations, New York, 1998.
OECD (Organization for Economic Co- operation and Development), Exposure to Radiation from Radioactivity in Building
Materials, (1979) (Report by a group of experts of the OECD Nuclear Energy Agency).
ICRP, Protection against Rn-222 at home and at work, Ann. ICRP 23 (2) (1994) 1–48 (ICRP publication 65; Ann ).
RPA, Naturally Occurring Radiation in the Nordic Countries: Recommendations, Statens stralskyddsinstitut, Stockholm,
M. Tufail, A. Nasim, J. Sabiha, H. Tehsin, Natural radioactivity hazards of building bricks fabricated from soil of two districts
of Pakistan, J. Radiol. Prot. 27 (2007) 481–492.